# Grade 35 (R56340) Titanium

Grade 35 titanium is a titanium alloy formulated for primary forming into wrought products. Cited properties are appropriate for the annealed condition. R56340 is the UNS number for this material. Additionally, the ASTM designation is Titanium Grade 35.

It has a fairly low ductility among wrought titaniums. In addition, it has a moderately high density and a moderately high tensile strength.

The graph bars on the material properties cards below compare grade 35 titanium to: wrought titaniums (top), all titanium alloys (middle), and the entire database (bottom). A full bar means this is the highest value in the relevant set. A half-full bar means it's 50% of the highest, and so on.

## Mechanical Properties

Elastic (Young's, Tensile) Modulus

110 *GPa* 16 *x 10 ^{6} psi*

Elongation at Break

5.6 *%*

Fatigue Strength

330 *MPa* 49 *x 10 ^{3} psi*

Poisson's Ratio

0.32

Reduction in Area

23 *%*

Shear Modulus

41 *GPa* 6.0 *x 10 ^{6} psi*

Shear Strength

580 *MPa* 85 *x 10 ^{3} psi*

Tensile Strength: Ultimate (UTS)

1000 *MPa* 150 *x 10 ^{3} psi*

Tensile Strength: Yield (Proof)

630 *MPa* 92 *x 10 ^{3} psi*

## Thermal Properties

Latent Heat of Fusion

420 *J/g*

Maximum Temperature: Mechanical

320 *°C* 610 *°F*

Melting Completion (Liquidus)

1630 *°C* 2960 *°F*

Melting Onset (Solidus)

1580 *°C* 2870 *°F*

Specific Heat Capacity

550 *J/kg-K* 0.13 *BTU/lb-°F*

Thermal Conductivity

7.4 *W/m-K* 4.3 *BTU/h-ft-°F*

Thermal Expansion

9.3 *µm/m-K*

## Electrical Properties

Electrical Conductivity: Equal Volume

1.1 *% IACS*

Electrical Conductivity: Equal Weight (Specific)

2.2 *% IACS*

## Otherwise Unclassified Properties

Base Metal Price

37 *% relative*

Density

4.6 *g/cm ^{3}* 280

*lb/ft*

^{3}Embodied Carbon

33 *kg CO _{2}/kg material*

Embodied Energy

530 *MJ/kg* 230 *x 10 ^{3} BTU/lb*

Embodied Water

170 *L/kg* 20 *gal/lb*

## Common Calculations

Resilience: Ultimate (Unit Rupture Work)

49 *MJ/m ^{3}*

Resilience: Unit (Modulus of Resilience)

1830 *kJ/m ^{3}*

Stiffness to Weight: Axial

13 *points*

Stiffness to Weight: Bending

35 *points*

Strength to Weight: Axial

61 *points*

Strength to Weight: Bending

49 *points*

Thermal Diffusivity

3.0 *mm ^{2}/s*

Thermal Shock Resistance

70 *points*

## Alloy Composition

Ti | 88.4 to 93 | |

Al | 4.0 to 5.0 | |

Mo | 1.5 to 2.5 | |

V | 1.1 to 2.1 | |

Fe | 0.2 to 0.8 | |

Si | 0.2 to 0.4 | |

O | 0 to 0.25 | |

C | 0 to 0.080 | |

N | 0 to 0.050 | |

H | 0 to 0.015 | |

res. | 0 to 0.4 |

All values are % weight. Ranges represent what is permitted under applicable standards.

## Followup Questions

## Similar Alloys

## Further Reading

Titanium Alloys: Modelling of Microstructure, Properties, and Applications, Wei Sha and Savko Malinov, 2009

ASTM B861: Standard Specification for Titanium and Titanium Alloy Seamless Pipe

ASTM B381: Standard Specification for Titanium and Titanium Alloy Forgings

ASTM B265: Standard Specification for Titanium and Titanium Alloy Strip, Sheet, and Plate

ASTM B348: Standard Specification for Titanium and Titanium Alloy Bars and Billets

Titanium and Titanium Alloys: Fundamentals and Applications, Christoph Leyens and Manfred Peters (editors), 2003

Titanium, 2nd ed., G. Lutjering and J. C. Williams, 2007